arXiv:1701.06921v1 [cond-mat.mtrl-sci] 24 Jan 2017

2 3 4

Department of Physics, Central Michigan University, Mount Pleasant MI, USA

Science of Advanced Materials Program, Central Michigan University, Mount Pleasant MI, USA

Department of Physics and Department of Chemistry, University of North Texas, Denton TX, USA

Dipartimento di Fisica, Informatica e Matematica, Universit´ a di Modena and Reggio Emilia, Via Campi 213/a, 41125 Modena, Italy 5 6 7

CNR-NANO Research Center S3, Via Campi 213/a, 41125 Modena, Italy

CNR-ISTM, Istituto di Scienze e Tecnologie Molecolari, I-20133 Milano, Italy

Materials Science, Electrical Engineering, Physics and Chemistry, Duke University, Durham NC, 27708 8

Center for Materials Genomics, Duke University, Durham, NC 27708, USA ?

corresponding: [email protected]

Abstract Tight-binding models provide a conceptually transparent and computationally efficient method to represent the electronic properties of materials. With AFLOWπ we introduce a framework for high-throughput first principles calculations that automatically generates tight-binding hamiltonians without any additional input. Several additional features are included in AFLOWπ with the intent to simplify the self-consistent calculation of Hubbard U corrections, the calculations of phonon dispersions, elastic properties, complex dielectric constants, and electronic transport coefficients. As examples we show how to compute the optical properties of layered nitrides in the AM N2 family, and the elastic and vibrational properties of binary halides with CsCl and NaCl structure. Keywords: High-throughput Calculations, Computer Simulations, Materials Databases 1. Introduction

Accelerated materials discovery is currently the focus of much infrastructure development both for experimental (see for instance Refs. [1–4]) and theoretical research [5–7]. The key components always involve robust data generation or collection, real time feedback and error control, curation and archival of the data, and post-processing tools for analysis and visualization. The ultimate goal is to discover relationships that may be hidden in the large data sets and possibly predict materials with improved specific functionalities. Preprint submitted to Elsevier

Flavors of density functional theory (DFT) usually form the basis for the generation of theoretical data since they provide reasonable transferability across different chemical compositions and structural themes at acceptable computational cost. Standard electronic structure packages such as Quantum Espresso [8] or VASP [9] are used as the engine of the calculations but an additional layer of software tools is needed to efficiently manage the high-throughput (HT) workflows. In addition, to streamline data generation, those software tools usually curate the data and prepare them for distribution in online electronic structure properties databases [10–13] that can be mined a posteriori.

January 25, 2017

are available online on the AFLOW.org repositories [11, 30, 31] (see http://www.aflow.org). With AFLOWπ we are complementing AFLOW with a minimalist software infrastructure that is easily portable, simple to use, and integrated with the AFLOW.org repositories. AFLOWπ has been initially developed for verification and testing purposes but has evolved into a modular software infrastucture that provides automatic workflows for the ab initio generation of tight-binding hamiltonians within the projected atomic orbital (PAO) scheme [32–34] and the self-consistent calculation of Hubbard U corrections within the ACBN0 approach [35]. In addition, workflows for the calculation of phonon dispersions with Hubbard U correction, the calculation of elastic constants, diffusive transport coefficients, and optical spectra are available. When possible, the code exploits the tight-binding hamiltonians as in Ref. [36].

Figure 1: The directory tree created by AFLOWπ during

the preparation of the calculation with in a PROJECT directory. Each SET contains the AFLOWpi directory with several auxiliary files discussed in the text. PROJECT and SET are substituted with specific values.

Several HT frameworks for electronic structure calculations were discussed in the literature. PYMATGEN [14] is the data generation software infrastructure behind the Materials Project database [10]. It is written in Python 2.7 using libraries such as Numpy and Scipy and exploits VASP and AbInit [15] as standard electronic structure engines. Many tools are available to study phase stability and phase diagrams. AiiDA [16] is an integrated software based on a paradigm involving automation, data, environment, and storage. It is written in Python 2.7 and revolves around relational databases for the overall design in addition to the storage component. For the automation component AiiDA involves workflows that use Quantum Espresso although other electronic structure codes are supported. In addition, scripting interfaces such ASE [17] can be used by AiiDA to control the workflow. ASE is paired with the Computational Materials Repository [18]. Additional HT software tools for density functional calculations are qmpy (associated with the Open Quantum Materials Database) [19] and the HT toolkit (HTTK associated with the Open Materials Database, http://httk.opendatabase.se); these software packages are written in Python and streamline electronic structure data generation. The framework AFLOW [20–27] is an efficient tool for highthroughput calculations with VASP. It is written in C++ and includes tools to create input files for Quantum Espresso, to deal automatically with supercells and fractional occupations, to perform symmetry analysis, and to evaluate several thermodynamical and thermal transport properties at different levels of approximation [28, 29]. Data generated with AFLOW

2. Software design and data organization AFLOWπ ’s design provides a simple, task oriented Python package to construct large sets of calculations from one or few input files for a specific ab initio engine and then to perform a workflow of tasks for each calculation in the set. The infrastructure is modeled on a simple and common modus operandi that involves prototypical input files (reference files) that are modified for desired tasks. The chosen workflow instructs AFLOWπ how to modify the reference files and guides the process of submitting, running, and monitoring all calculations. The software is implemented in Python 2.7 (using the Python standard library and Numpy, Scipy, CIFfile, and Matplotlib). The systematic use of regular expression (re module) to parse and modify the input and output files according the specific workflow makes the software very portable and expandable to a variety of electronic structure engines and tools. Currently, AFLOWπ encapsulates pw.x and several postprocessing software from the Quantum Espresso package [8] as well as ElaStic [37]. In addition it uses features of findsym [38]. The generation and manipulation of the TB Hamiltonians is done with the engine PAOπ [39]. The calculations and the resulting data are organized according to the layer structure adopted by AFLOW [30]. The first layer in the directory hierarchy is the 2

Project layer that can contain multiple instances of the next layer, the Set layer. The directories for the individual calculation pipelines in the set are named PROJECT SET XXXX with PROJECT being the project name, SET being the name of the set and XXXX being the index of the calculation (See Figure 1). Each calculation pipeline receives a unique identifier to keep track of each pipe of calculations during setup and runtime as well as for storage and retrieval of the results. The identifier is constructed as a CRC64 hash [40], which is a unique 16 character string representing the initial ab initio engine input file for each calculation pipeline. The input file is first cleaned of commented out content and unnecessary whitespace, then lines of text are sorted alphabetically. Cleaning and sorting is necessary to ensure that extra whitespace or the ordering of the parameters will not change the value of the hash. Files for each task, or step, in each calculation pipeline are designated by ID XX where XX is the step number and ID is the identifier for that calculation pipeline. An input for the first step in a pipeline with the identifier 20b8c6f83a2ca9b would read c20b8c6f83a2ca9b 01.in. Files and directories within each calculation’s directory that are considered unneeded after runtime, often referred to as scratch, such as Python scripts generated by AFLOWπ , cluster submission files, and temporary files of the ab initio engine have a prepended underscore. For example, the filename of the Python executable for the second step in that pipeline would be c20b8c6f83a2ca9b 02.py. AFLOWπ modularizes the calculation pipelines by separating each task into its own executable. When a task is completed, the next task is initiated and so on until the pipeline completes. The location of the directory for each calculation pipeline is preserved for all tasks the user issues for the set. All files needed to perform the tasks as well as all files generated by the tasks are stored in the folder pertaining to the individual calculation pipeline in order to ensure control and transferability.

itor the workflow especially for resuming or expanding the calculations. AFLOWπ will run as a cluster job submission (currently PBS, http://pbsworks.com) or as a local process on systems without a cluster queue. The user has the freedom to choose how the steps in the workflows of the calculations are grouped in terms of cluster submissions. Specific mechanisms for auto-restart and both manual and automatic error control have been implemented to manage the full set of calculations at once. The restart mechanism keeps track of the time a cluster job has been running and prepares calculations so that the electronic structure engine exits cleanly before the wall-time runs out. A wall-time buffer with a default of 10% of the total wall-time request allows time to save data to disk and, if local scratch option is used, for the temporary files in the local scratch diskspace to be copied to the global scratch. After cleaning up temporary files, the command to resubmit the cluster job is given and then the job exits. There are several locking mechanisms in place to ensure that there is no wasted calculation time. In addition to auto restarting, if there are major failures of the electronic structure engine, the user can load a calculation set and filter only the jobs where there were errors causing the execution pipeline to stop at a certain point and check what kind of errors occurred, if any. Calculations that failed can be filtered into a subset. Certain actions can be taken to help the subset to complete. AFLOWπ ’s source code includes documentation import AFLOWpi session = AFLOWpi.prep.init(’mHT TB’, ,→ ’III−V’,config=’./mHT TB.config’) allvars ={} allvars .update( AFLOWPI A = (’Al’,’Ga’,’In’), AFLOWPI B = (’P’,’As’,’Sb’),) calcs = session. scfs ( allvars , ’mHT TB.ref’) calcs . vcrelax () tb ham = calcs.tight binding() tb ham.dos() tb ham.bands() tb ham.plot.bands(DOSPlot=’APDOS’) calcs .acbn0() tb ham = calcs.tight binding() tb ham.dos() tb ham.bands() tb ham.plot.bands(DOSPlot=’APDOS’) calcs .submit()

Within each Set, AFLOWπ creates a directory named AFLOWpi that contains a master runtime log of the session, a copy of the configuration file used in the session, a summary log with relevant information from the output of every calculation within the set, as well as the loadable calculation files (LCFs). In order to ensure data provenance AFLOWpi includes mandatory information to be provided at the beginning of the data generation process. Each calculation pipeline has its own LCF that are pickled and used to control and mon-

Figure 2: Workflow to compute total energies, tight-binding

hamiltonians, band structures, densities of states (DOS), and atom projected DOS with and without ACBN0 for AlP, GaP, InP, AlAs, GaAs, AlSb, GaSb, and InSb. The construction of this workflow is discussed in the text.

3

strings written in the Google Python docstring format for readability. These docstrings are located at the beginning of each function or class. AFLOWπ documentation is generated via the Sphinx Python package. Sphinx can be used to parse source code written in Python, C, C++ as well as several other programming languages to automatically generate user documentation from docstrings. We use Sphinx to generate LATEX documentation for AFLOWπ as well as a searchable html documentation.

investigation of such systems. ACBN0 only demands computational resources comparable to regular LDA or PBE calculations. We have extensively investigated the improvements and the limits of ACBN0 calculation in Refs. [41, 42]. Overall, ACBN0 delivers better accuracy for lattice parameters and bulk moduli, improves the energy band gap on semiconductors and insulators as well as the relative position of occupied d-manifolds in transition metal oxides, and optimizes the phonon dispersions and associated thermal transport properties.

3. Generation of tight-binding hamiltonians

Electronic Band Structure: GaP

5

Density of States (States/eV) Ga P

4

Theory and applications of the methodology used by AFLOWπ to generate tight-binding (TB) hamiltonians for first principles plane-wave pseudopotential calculations have been discussed in Refs. [32–34]. Our implementation does not require any additional input with respect to the electronic structure calculations and provides the real space representation of the TB matrix in self-contained XML format. The sparse TB matrix is represented on a grid as Hα,β (r) and can be easily Fourier transformed into

3 2

E(eV)

1 0 1 2 3 4 5Γ

X

W

K

Γ

L

U

W

L

K|U X

arbitrary units

Band structure and DOS plot generated by AFLOW π using the tight-binding (TB) hamiltonian for GaP r without ACBN0. The workflow in Figure 2 has been used to and diagonalized to determine the full energy disper- obtain this result. TB hamiltonians can be post-processed to perform investigations of the energy dispersions away sions, En (k), with the desired level of resolution in from symmetry lines or interpolations in reciprocal space reciprocal space or to compute additional properties at minimal computational cost.

Hα,β (k) =

X

Figure 3:

exp (ik · r) Hα,β (r) ,

associated with derivatives in reciprocal space (linear momenta, and effective masses). The real space representation can also be used directly. We have recently applied these methodologies to study diffusive and ballistic transport as well as the optical properties in the independent particles approximation [36].

Electronic Band Structure: GaP

5

Density of States (States/eV) Ga P

4 3 2

E(eV)

1

4. ACBN0 calculations

0 1 2

The TB representation of the electronic structure can be exploited to efficiently compute two-electron integrals for the development of local exchange functionals. AFLOWπ implements the direct and self-consistent evaluation of the on-site Hubbard U correction that greatly improves the accuracy of standard DFT calculations [35]. Due to the accurate TB representation, the evaluation of the U parameters for atoms in different chemical environments or close to topological defects becomes trivial and AFLOWπ facilitates the

3 4 5Γ

X

W

K

Γ

L

U

W

L

K|U X

arbitrary units

Figure 4: As in Figure 3 but computed with ACBN0. The

main improvements for this specific example are associated with a more realistic energy gap, and changes in the dispersion curves near X and L in the conduction band. The top valence bands are also slightly more dispersed.

4

Table 1: Hubbard U corrections (in eV) computed self-consistently for III-V semiconductors with the workflow discussed

˚ in the text. The theoretical lattice parameters a0L and aU L (in A) are computed with and without ACBN0 respectively. Energy gaps (in eV) for Γ − Γ, Γ − X and Γ − L are calculated with and without ACBN0. Experimental values are shown in parentheses.

UIII UV a0L aU L E0Γ EUΓ E0X EUX E0L EUL

AlP 0.01 2.31 5.49 (5.46) 5.44 (5.46) 3.1 (3.6) 3.9 (3.6) 1.3 (2.5) 2.1 (2.5) 2.7 (2.5) 3.3 (2.5)

AlAs 0.08 2.12 5.74 (5.66) 5.67(5.66) 1.8 (3.0) 2.5 (3.0) 1.5 (2.2) 1.9 (2.2) 1.7 (2.4) 2.6 (2.4)

AlSb 0.17 1.11 6.23 (6.13) 6.17(6.13) 1.2 (2.3) 1.7 (2.3) 1.3 (1.7) 1.5 (1.7) 1.3 (2.3) 1.5 (2.3)

GaP 20.00 1.87 5.53 (5.45) 5.48(5.45) 1.3 (2.8) 1.9 (2.8) 2.1 (2.3) 2.1 (2.3) 1.4 (2.7) 1.8 (2.7)

GaAs 20.01 1.75 5.79 (6.05) 5.73(6.05) 0.0 (0.8 ) 0.5 (0.8) 1.6 (1.1) 1.9 (1.1) 0.7 (0.9) 1.1 (0.9)

InP 14.97 0.00 5.97 (5.86) 5.91 (5.86) 0.4 (1.4) 1.0 (1.4) 1.8 (2.4) 2.3 (2.4) 1.1 (2.0) 1.8 (2.0)

Table 2: Value of the energy gaps and U corrections (in eV) computed with ACBN0 for AM N2 compounds.

U(A) U(M) U(N) Eg

SrTiN2 0.04 0.28 3.09 1.25

BaTiN2 3.69 0.29 2.93 1.02

SrZrN2 0.04 0.28 3.09 1.85

BaZrN2 4.32 0.20 2.80 1.58

SrHfN2 0.05 0.13 3.06 2.21

BaHfN2 4.40 0.15 2.80 1.87

Table 3: Elastic constants computed for a set of alkali halides. We determined the U corrections with ACBN0 and

compared with the experimental data from Ref. [43] and data from Ref. [44]. Structural parameters and U values are in Table 4.

LiF

LiCl

NaF

NaCl

KF

KCl

Cij ( GPa) C11 C12 C44 C11 C12 C44 C11 C12 C44 C11 C12 C44 C11 C12 C44 C11 C12 C44

ACBN0 113.6 50.6 66.2 51.5 23.9 27.1 101.1 24.8 29.4 51.2 13.4 13.9 60.9 14.9 14.5 37.6 6.8 7.2

5

PBE 111.5 46.3 60.4 52.1 21.8 24.9 95.9 22.2 26.4 49.2 12.0 12.3 60.1 14.1 13.6 36.2 6.3 6.6

EXP 113.9 47.6 63.6 60.7 22.7 26.9 108.9 22.9 28.9 57.3 11.2 13.3 75.7 13.5 13.3 40.9 7.0 6.2

Model 104.6 42.4 70.8 66.6 20.9 24.6 97.6 22.9 29.9 54.5 11.2 11.6 85.0 14.7 17.1 53.8 5.4 8.3

Table 4: Structural parameters (in ˚ A) and U corrections (in eV) computed with ACBN0 for selected AX alkali halides

using the NaCl structure

U(A) U(X) aL

LiF 0.14 11.41 3.99

LiCl 0.04 6.31 5.06

LiBr 0.01 5.49 5.41

NaF 0.19 11.95 4.60

NaCl 0.02 6.95 5.57

5. Installation and data generation

NaBr 0.02 5.97 5.89

KF 0.17 12.77 5.32

KCl 0.03 7.29 6.24

KBr 0.02 6.27 6.55

for the atomic species are substituted with the variables AFLOWPI A and AFLOWPI B. That input combined with the list of chemical substitutions is processed by AFLOWπ in order to prepare a pipeline of calculations starting with the determination of the ground state potential (session.scfs), the structural relaxations (calcs.vcrelax), and the generation of the TB hamiltonian (calcs.tight binding) including plots for the densities of states and the band structures. Then the workflow continues with the self-consistent calculation of the Hubbard corrections (calcs.acbn0) before recalculating a new TB hamiltonian and new plots. At the end of the user’s AFLOWπ script, the command calcs.submit must be included to run the calculation workflow (see Figure 2). In Figs. 3 and 4, we show plots generated by AFLOWπ before and after the ACBN0 cycle. It is interesting to pinpoint the corrections of the band gap and the modification of the dispersion relationships (the Hubbard corrections determined running this workflow are in Table 1). All the tight-binding hamiltonians are stored as XML files and can be distributed independently. We stress the fact that the energy dispersion En (k) can be computed with ab initio accuracy.

The minimalist style of AFLOWπ makes it easy to install the software. One command to download the source code from its repository online, and two commands to enter the directory and to install AFLOWπ as an importable Python package. The setup.py in the base directory of the AFLOWπ source code tree is executed to build and make it importable in Python scripts. All the commands can be run interactively through any Python shell. Currently AFLOWπ includes three basic submodules: prep, run, scfuj to perform the basic calculations including ACBN0 and the generation of tight-binding hamiltonians. The regular expressions for interacting with a specific electronic structure engine (pw.x for instance) are stored separately. In addition, the plot, aflowlib, db, retr modules can be used to extract, post-process, and export the computed quantities. The distribution also includes the pseudo module for pseudo-potential testing. A detailed description of all the methods is included in the distribution as well as practical examples. A simple interface class allows for easy customization of calculation workflows using methods to instruct AFLOWπ to prepare the specific tasks. Several styles may be used in AFLOWπ to define the The construction of a workflow starts with the calculations in a set. The first style is based on the command AFLOWpi.prep.init() which initiates the cartesian product of two lists (as in Figure 2). The AFLOWπ session and requires a project name and second style, labelled “zip mode”, generates all the enthe name of the configuration file as input. Spec- tries by taking, in order, the corresponding entries in ifying sets within a project is optional but highly the keywords lists (see Section 7.2). In addition, calcurecommended. AFLOWpi.prep.init() returns a ses- lation sets can be formed from a list of one or more insion object which has methods to form the calculation put filenames for the electronic structure engine (these sets. When one of the methods of the session object can be completed appropriately with the missing variis called, it returns a “calculation set” object. The ables). calculation set object contains methods to construct workflows which add tasks to be done for each calculation in the set. Let assume we plan to generate the PAO-TB hamiltonians for the III-V semiconductors (AlP, GaP, InP, AlAs, GaAs, AlSb, GaSb, and InSb) from the electronic structure generated without and with the ACBN0 approach. In a prototypical reference input file (e.g. mHT TB.ref) the labels

6. Data retrieval and exporting AFLOWπ extracts and monitors data such as energy, structure, atomic positions, total force, total stress, and automatically records it in the summary.log file in the calculation set’s AFLOWpi directory. Quanti6

ties such as those listed above can be extracted for We report data for AM N2 compounds in Table 2 and a given step of the calculation pipeline using the in Figure 6. Among the AM N2 compositions, the AFLOWpi.retr module. compounds containing Ti have absorption edges below the Shockley-Queisser limit of 1.34 eV; the compounds In addition, results can be packaged for the online containing Hf and Zr exceed such a limit but seem porepository www.aflow.org by adding tentially interesting as end points of A(Ti,M )N2 alloys with M =Zr and Hf where tuning of the band gap can AFLOWpi.aflowlib.export(’export example’, lead to improved photovoltaics potentials. set name=’III−V’, config=’./mHT TB.config’)

to the workflow.

7.2. Phonons and elastic constants

AFLOWπ also includes post-processing routines to compute and plot the radial distribution function, compare the energetics of different distortions, generate CIF files, and perform symmetry analysis.

In order to show how the calculations of phonon dispersions and of the elastic constants can be performed in AFLOWπ we analyzed a small chemical space of alkali halides AX with (A=Li, Na, K and X=F, Cl, Br) with the NaCl and the CsCl structures. The workflow is in Figure 7: notice the use of the zip mode to specify the chemical space and the use of two reference files for the NaCl and CsCl structure, respectively. Elastic constants are computed solely on the NaCl structure.

7. Examples 7.1. Optical (and transport) properties

Under normal conditions, alkali halides have NaCl or B1-type crystal structure, but they transform under moderate pressure to the CsCl or B2-type structure. There has been much work done on thermal conductivity during the phase transition of alkali halides: Averkin [51] found that the phase transition completely eliminates the influence of the elastic anisotropy on the thermal conductivity, as well as its dependence on pressure. In that paper an empirical relation was also established between elastic anisotropy and thermal conductivity. However, Slack [52] concluded that there is no need to invoke the elastic anisotropy to explain thermal conductivity differences. He noticed that NaCl structure compounds have a higher thermal conductivity ratio than CsCl ones by about a factor of two import AFLOWpi and conjectured a large increase in the Gr¨ uneisen pasession = AFLOWpi.prep.init(’Transport’, ’Si’, ,→ config=’./transport. config ’ ) rameter as the co-ordination number changes from six calcs = session. from file ( ’transport. in ’ ) to eight. Our results indicate, however, that a major calcs . vcrelax () # get PAO−TB hamiltonian contribution to the change in the thermal conductivcalcs TB = calcs.tight binding () ity is related to the average sound velocity reduction # optical and transport properties calcs TB.epsilon () in CsCl structure with respect to the NaCl structure. calcs TB.transport(temperature=[300,400]) In Figure 8 we report, as an example, phonon disper# plot optical and transport properties sions automatically generated by AFLOWπ using a calcs TB.plot.transport() calcs TB.plot. epsilon () finite difference method. We did not observe significalcs .submit() cant changes using the ACBN0 approach with respect Figure 5: Workflow to compute optical (and transport) prop- to the PBE calculations, and we choose to report seerties for layered nitrides with chemical formula AM N2 . lected ACBN0 data as an example. Layered nitrides with chemical formula AM N2 were studied earlier from the point of view of thermoelectric potentials and superconductivity [45–50]. As an example we analyze the same chemical space (A=Sr, Ba and M=Ti, Zr, Hf) from the point of view of the electronic transport in the constant relaxation time approximation and the optical properties within the independent electronic approximation. Using well converged basis sets and k-space sampling (see Ref. [45] for computational details), we have determined the electrical conductivity, the Seebeck coefficient, and the the complex dielectric functions with and without ACBN0. The workflow is in Figure 5.

The complex dielectric constant is computed within the independent particle approximation with and without the The elastic constants of alkali halides are important as ACBN0 correction The comments show how to compute they are closely related to the ionic binding force in the electronic transport as discussed in Ref. [36]. the crystal [44]. There are several phenomenological

7

²: BaHfN2 25

²: HfN2 Sr

²1 ²2

²1 ²2

35

20

30 25

² (au)

² (au)

15

10

20 15 10

5 5 00.5

1.0

1.5

2.0

2.5

ω (eV)

3.0

3.5

4.0

00.5

4.5

1.0

1.5

²: BaN2 Zr 25

2.0

2.5

ω (eV)

3.0

3.5

4.0

4.5

3.0

3.5

4.0

4.5

²: N2 SrZr

²1 ²2

35

²1 ²2

30 25

² (au)

² (au)

20

15

20 15

10 10 5

00.5

5 1.0

1.5

2.0

2.5

ω (eV)

3.0

3.5

4.0

00.5

4.5

1.0

1.5

2.0

2.5

ω (eV)

Figure 6: Complex dielectric constant generated by AFLOWπ using the tight-binding hamiltonian as in Ref. [36] for

AM N2 compounds with A=Ba, Sr and M =Hf, Zr. The titanates exhibit absorption edges just above 1eV. The workflow in Figure 5 has been used to obtain this result. Additional data including the correction to the band gap provided by ACBN0 are in Table 2.

ciples calculations with and without ACBN0, experimental data, and results from Ref. [44]. Our results improve the agreement with experimental data with respect to the model in Ref. [44] and indicate the sensitivity of the elastic constants to the choice of the computational method.

models to determine the elastic constants: in the central force model [53], the elastic constants are given by the sum of the terms due to long range and short range central forces. This model leads to a Cauchy relation C12 = C44 , which is not true experimentally. The degree to which this Cauchy relation is not satisfied is a measure of the importance of many-body forces in lattice dynamics of the alkali halide which Lowdin [54] has found to exist. The breathing shell model [55] includes many-body forces and makes a prediction C12 < C44 in alkali halides. Mahan [44] studied the effect of induced polarization on phonon modes at long wavelength and introduced a polarization term in the central force model predicting C12 > C44 . Experimentally the deviation is found in both directions. We report in Table 3 the comparison between first prin-

8. Conclusions We have presented here a minimalist high-throughput software infrastructure that, in addition to organizing and controlling the computational workflow, facilitates the generation of tight-binding Hamiltonians to represent accurately the electronic properties with ab initio accuracy. AFLOWπ exploits the tight-binding formal8

Phonon Dispersion and DOS: BrRb

140

Frequency (cm−1 )

120 100 80 60 40 20 0Γ

X

W

K

Γ

L

U

W

L

Phonon Dispersion and DOS: BrRb

K|U X Density of States (arb. units)

120

Frequency (cm−1 )

100 80 60 40 20 0Γ

X

M

R

Γ

Phonon Dispersion and DOS: ClK

X|M

R Density of States (arb. units)

X|M

R Density of States (arb. units)

Frequency (cm−1 )

200 150 100 50 0Γ

X

M

R

Γ

Phonon Dispersion and DOS: ClK

Frequency (cm−1 )

200 150 100 50 0Γ

X

W

K

Γ

L

U

W

L

K|U X Density of States (arb. units)

Figure 8: Phonon branches and vibrational density of states for CsCl and NaCl structure of RbBr and KCl at equilibrium lattice parameters. We used the workflow in Figure 7.

9

ism to compute electronic transport and optical properties within the independent particle approximation. Three examples were used to illustrate the features of AFLOWπ (1) the calculation of the band structure of III-V semiconductors with and without the ACBN0 correction, (2) the study of the complex dielectric constant of AM N2 (A=Sr, Ba and M =Ti, Zr, Hf), and (3) the phonon dispersions and the elastic constants of binary halides (AX with A=Li, Na, K and X=F, Cl, Br). We found that A(Ti,M )N2 alloys with M =Zr and Hf may have potential for photovoltaic applications. In addition, we justified the dramatic changes in thermal conductivity occurring at the transition between NaCl and CsCl structure in terms of sound velocity. The code, including the examples presented in this paper, is available at www.aflow.org/aflowpi.

import AFLOWpi # Create AFLOWpi session ses CsCl = AFLOWpi.prep.init(’Halide’, ’CsCl’, config=’./phonon.config’) ses NaCl = AFLOWpi.prep.init(’Halide’, ’NaCl’, config=’./phonon.config’) # Generate a calculation set from a reference input file allvars ={”\ AFLOWPI\ A ”:(”Li”,”Na”,”K”,), ”\ AFLOWPI\ B ”:(”F”,”Cl”,”Br”,”I”),} CsCl = ses CsCl.scfs( allvars , ’CsCl.ref ’ ,) NaCl = ses NaCl.scfs(allvars , ’NaCl.ref’ ,) #do a vc−relax CsCl.vcrelax() NaCl.vcrelax() # change the thresholds in the input files # changing input for a step are called after # the call for the step . the change calcs # below affect the vc−relax above CsCl.change input(”&control”,”etot conv thr”,”1.0D−5”) CsCl.change input(”&control”,”forc conv thr”,”1.0D−4”) CsCl.change input(”&electrons”,”conv thr”,”1.0D−16”) NaCl.change input(”&control”,”etot conv thr”,”1.0D−5”) NaCl.change input(”&control”,”forc conv thr”,”1.0D−4”) NaCl.change input(”&electrons”,”conv thr”,”1.0D−16”) #do another relax just to be safe CsCl.vcrelax() NaCl.vcrelax() #do phonon calculations with 2x2x2 supercell CsCl.phonon(mult jobs=True,nrx1=3,nrx2=3,nrx3=3,innx=2, ,→ de=0.003,LOTO=True,field strength=0.003, ,→ disp sym=True,atom sym=False,) NaCl.phonon(mult jobs=True,nrx1=3,nrx2=3,nrx3=3,innx=2, ,→ de=0.003,LOTO=True,field strength=0.003, ,→ disp sym=True,atom sym=False,) #plot the phonons NaCl.plot.phonon(postfix=’NaCl’) CsCl.plot.phonon(postfix=’CsCl’) # do the elastic constants with the ElaStic Package # Install : http:// exciting−code.org/elastic NaCl.elastic (mult jobs=False,num dist=10,eta max=0.001) #do acbn0 to do phonon with self−consistently #determined Hubbard U. Changing the cell while #converging the U should be done with caution. NaCl.scfuj(relax=’vc−relax’) CsCl.scfuj(relax=’vc−relax’) NaCl.elastic (mult jobs=False,num dist=10,eta max=0.001) NaCl.phonon(mult jobs=True,nrx1=3,nrx2=3,nrx3=3,innx=2, ,→ de=0.003,LOTO=True,field strength=0.003, ,→ disp sym=True,atom sym=False,) CsCl.phonon(mult jobs=True,nrx1=3,nrx2=3,nrx3=3,innx=2, ,→ de=0.003,LOTO=True,field strength=0.003, ,→ disp sym=True,atom sym=False,) CsCl.plot.phonon(postfix=’CsCl acbn0’) NaCl.plot.phonon(postfix=’NaCl acbn0’) # submit the calcs to run calcs .submit()

9. Acknowledgments We are grateful to the High Performance Computing Center at Michigan State University and the Texas Advanced Computing Center at the University of Texas Austin. The members of the AFLOW Consortium (http://www.aflow.org) acknowledge support by DOD-ONR (N00014-13-1-0635, N00014-11-1-0136, N00014-15-1-2863). The authors also acknowledge Duke University — Center for Materials Genomics — and the CRAY corporation for computational support.

Bibliography [1] R. Potyrailo, K. Rajan, K. Stoewe, I. Takeuchi, B. Chisholm, and H. Lam, Combinatorial and HighThroughput Screening of Materials Libraries: Review of State of the Art, ACS Combinatorial Science 13, 579–633 (2011). [2] K. Rajan, Combinatorial Materials Sciences: Experimental Strategies for Accelerated Knowledge Discovery, Annual Review of Materials Research 38, 299–322 (2008).

Figure 7: Workflow to compute phonon dispersion with and

without ACBN0 for few alkali halides in NaCl and CsCl structure. For the NaCl set of calculations also the elastic constants are computed and compared with the experimental data in Table 3.

[3] I. Takeuchi, C. J. Long, O. O. Famodu, M. Murakami, J. Hattrick-Simpers, G. W. Rubloff, M. Stukowski, and K. Rajan, Data management and visualization of x-ray diffraction spectra from thin film ternary composition spreads, Review of Scientific Instruments 76, 062223 (2005). [4] A. G. Kusne, T. Gao, A. Mehta, L. Ke, M. C. Nguyen, K.-M. Ho, V. Antropov, C.-Z. Wang, M. J. Kramer, C. Long, and I. Takeuchi, On-the-fly machine-learning

10

[14] S. P. Ong, W. D. Richards, A. Jain, G. Hautier, M. Kocher, S. Cholia, D. Gunter, V. L. Chevrier, K. A. Persson, and G. Ceder, Python Materials Genomics (pymatgen): A robust, open-source python library for [5] S. Curtarolo, G. L. W. Hart, M. Buongiorno Nardelli, materials analysis, Comput. Mater. Sci. 68, 314–319 N. Mingo, S. Sanvito, and O. Levy, The high(2013). throughput highway to computational materials design, [15] X. Gonze, J.-M. Beuken, R. Caracas, F. Detraux, Nat. Mater. 12, 191–201 (2013). M. Fuchs, G.-M. Rignanese, L. Sindic, M. Verstraete, G. Zerah, F. Jollet, M. Torrent, A. Roy, M. Mikami, [6] D. Morgan, G. Ceder, and S. Curtarolo, HighP. Ghosez, J.-Y. Raty, and D. C. Allan, First-principles throughput and data mining with ab initio methods, computation of material properties: the ABINIT softMeasurement Science and Technology 16, 296 (2005). ware project, Comput. Mater. Sci. 25, 478–492 (2002). for high-throughput experiments: search for rare-earthfree permanent magnets, Scientific Reports 4, 6367 EP– (2014).

[7] S. Curtarolo, D. Morgan, and G. Ceder, Accuracy of [16] G. Pizzi, A. Cepellotti, R. Sabatini, N. Marzari, and ab initio methods in predicting the crystal structures B. Kozinsky, AiiDA: automated interactive infrastrucof metals: A review of 80 binary alloys, Calphad 29, ture and database for computational science, Comput. 163–211 (2005). Mater. Sci. 111, 218–230 (2016). [8] P. Giannozzi, S. Baroni, N. Bonini, M. Calandra, [17] S. R. Bahn and K. W. Jacobsen, An object-oriented scripting interface to a legacy electronic structure code, R. Car, C. Cavazzoni, D. Ceresoli, G. L. Chiarotti, Comput. Sci. Eng. 4, 56–66 (2002). M. Cococcioni, I. Dabo, A. Dal Corso, S. de Gironcoli, S. Fabris, G. Fratesi, R. Gebauer, U. Gerstmann, [18] D. D. Landis, J. S. Hummelshøj, S. Nestorov, J. GreeC. Gougoussis, A. Kokalj, M. Lazzeri, L. Martinley, M. Dulak, T. Bligaard, J. K. Nørskov, and K. W. Samos, N. Marzari, F. Mauri, R. Mazzarello, S. Paolini, Jacobsen, The Computational Materials Repository, A. Pasquarello, L. Paulatto, C. Sbraccia, S. Scandolo, Comput. Sci. Eng. 14, 51–57 (2012). G. Sclauzero, A. P. Seitsonen, A. Smogunov, P. Umari, and R. M. Wentzcovitch, QUANTUM ESPRESSO: a [19] S. Kirklin, J. E. Saal, B. Meredig, A. Thompson, J. W. modular and open-source software project for quantum Doak, M. Aykol, S. R¨ uhl, and C. Wolverton, The Open simulations of materials, J. Phys.: Condens. Matter 21, Quantum Materials Database (OQMD): assessing the 395502 (2009). accuracy of DFT formation energies, Npj Computational Materials 1, 15010 EP– (2015). [9] G. Kresse and J. Furthm¨ uller, Efficiency of ab-initio total energy calculations for metals and semiconductors [20] S. Curtarolo, W. Setyawan, G. L. W. Hart, M. Jahn´atek, R. V. Chepulskii, R. H. Taylor, S. Wang, using a plane-wave basis set, Comput. Mater. Sci. 6, J. Xue, K. Yang, O. Levy, M. J. Mehl, H. T. Stokes, 15–50 (1996). D. O. Demchenko, and D. Morgan, AFLOW: An automatic framework for high-throughput materials discov[10] A. Jain, S. P. Ong, G. Hautier, W. Chen, W. D. ery, Comput. Mater. Sci. 58, 218–226 (2012). Richards, S. Dacek, S. Cholia, D. Gunter, D. Skinner, G. Ceder, and K. a. Persson, The Materials Project: [21] W. Setyawan and S. Curtarolo, High-throughput elecA materials genome approach to accelerating materials tronic band structure calculations: Challenges and innovation, APL Mater. 1, 011002 (2013). tools, Comput. Mater. Sci. 49, 299–312 (2010). [11] S. Curtarolo, W. Setyawan, S. Wang, J. Xue, K. Yang, [22] K. Yang, C. Oses, and S. Curtarolo, Modeling OffR. H. Taylor, L. J. Nelson, G. L. W. Hart, S. SanStoichiometry Materials with a High-Throughput Abvito, M. Buongiorno Nardelli, N. Mingo, and O. Levy, Initio Approach, Chem. Mater. 28, 6484–6492 (2016). AFLOWLIB.ORG: A distributed materials properties repository from high-throughput ab initio calculations, [23] O. Levy, M. Jahn´atek, R. V. Chepulskii, G. L. W. Hart, and S. Curtarolo, Ordered Structures in Rhenium BiComput. Mater. Sci. 58, 227–235 (2012). nary Alloys from First-Principles Calculations, J. Am. Chem. Soc. 133, 158–163 (2011). [12] M. Scheffler, C. Draxl, and Computer Center of the Max-Planck Society, Garching, The NoMaD Reposi- [24] O. Levy, G. L. W. Hart, and S. Curtarolo, Structure tory, http://nomad-repository.eu (2014). maps for hcp metals from first-principles calculations, Phys. Rev. B 81, 174106 (2010). [13] P. Scherpelz, M. Govoni, I. Hamada, and G. Galli, Implementation and Validation of Fully Relativistic [25] O. Levy, G. L. W. Hart, and S. Curtarolo, Uncovering Compounds by Synergy of Cluster Expansion and HighGW Calculations: Spin-Orbit Coupling in Molecules, Throughput Methods, J. Am. Chem. Soc. 132, 4830– Nanocrystals, and Solids, Journal of Chemical Theory 4833 (2010). and Computation 12, 3523–3544 (2016).

11

[26] G. L. W. Hart, S. Curtarolo, T. B. Massalski, [36] P. D’Amico, L. Agapito, A. Catellani, A. Ruini, and O. Levy, Comprehensive Search for New Phases S. Curtarolo, M. Fornari, M. Buongiorno Nardelli, and and Compounds in Binary Alloy Systems Based on A. Calzolari, Accurate ab initio tight-binding HamiltoPlatinum-Group Metals, Using a Computational Firstnians: Effective tools for electronic transport and optiPrinciples Approach, Phys. Rev. X 3, 041035 (2013). cal spectroscopy from first principles, Phys. Rev. B 94, 165166 (2016). [27] O. Isayev, D. Fourches, E. N. Muratov, C. Oses, K. Rasch, A. Tropsha, and S. Curtarolo, Materials Car- [37] R. Golesorkhtabar, P. Pavone, J. Spitaler, P. Puschnig, tography: Representing and Mining Materials Space and C. Draxl, ElaStic: A tool for calculating secondUsing Structural and Electronic Fingerprints, Chem. order elastic constants from first principles, Comput. Mater. 27, 735–743 (2015). Phys. Commun. 184, 1861–1873 (2013). [28] P. Nath, J. J. Plata, D. Usanmaz, R. Al Ra- [38] H. T. Stokes and D. M. Hatch, FINDSYM: program hal Al Orabi, M. Fornari, M. Buongiorno Nardelli, for identifying the space-group symmetry of a crystal, C. Toher, and S. Curtarolo, High-throughput predicJ. Appl. Cryst. 38, 237–238 (2005). tion of finite-temperature properties using the quasiharmonic approximation, Comput. Mater. Sci. 125, [39] M. Buongiorno Nardelli, PAOπ: a python utility to construct and operate on Hamiltonians from the Pro82–91 (2016). jections of DFT wavefunctions on Atomic Orbital [29] C. Toher, J. J. Plata, O. Levy, M. de Jong, M. D. bases, in preparation . Asta, M. Buongiorno Nardelli, and S. Curtarolo, Highthroughput computational screening of thermal conduc- [40] W. W. Peterson and D. T. Brown, Cyclic Codes for Error Detection, Proceedings of the IRE 49, 228–235 tivity, Debye temperature, and Gr¨ uneisen parameter (1961). using a quasiharmonic Debye Model, Phys. Rev. B 90, 174107 (2014). [41] P. Gopal, M. Fornari, S. Curtarolo, L. A. Agapito, L. S. I. Liyanage, and M. Buongiorno Nardelli, Im[30] R. H. Taylor, F. Rose, C. Toher, O. Levy, K. Yang, proved predictions of the physical properties of Zn- and M. Buongiorno Nardelli, and S. Curtarolo, A RESTCd-based wide band-gap semiconductors: A validation ful API for exchanging Materials Data in the of the ACBN0 functional, Phys. Rev. B 91, 245202 AFLOWLIB.org consortium, Comput. Mater. Sci. 93, (2015). 178–192 (2014). [31] C. E. Calderon, J. J. Plata, C. Toher, C. Oses, [42] M. Shishkin and H. Sato, Self-consistent parametrizaO. Levy, M. Fornari, A. Natan, M. J. Mehl, G. L. W. tion of DFT + U framework using linear response apHart, M. Buongiorno Nardelli, and S. Curtarolo, The proach: Application to evaluation of redox potentials of AFLOW standard for high-throughput materials scibattery cathodes, Phys. Rev. B 93, 085135 (2016). ence calculations, Comput. Mater. Sci. 108 Part A, [43] J. T. Lewis, A. Lehoczky, and C. V. Briscoe, Elastic 233–238 (2015). Constants of the Alkali Halides at 4.2K, Phys. Rev. [32] L. A. Agapito, A. Ferretti, A. Calzolari, S. Curtarolo, 161, 877–887 (1967). and M. Buongiorno Nardelli, Effective and accurate representation of extended Bloch states on finite Hilbert [44] G. D. Mahan, Elastic constants of alkali halides: Multipole expansion, Phys. Rev. B 29, 5849–5858 (1984). spaces, Phys. Rev. B 88, 165127 (2013). [33] L. A. Agapito, S. Ismail-Beigi, S. Curtarolo, [45] R. Al Rahal Al Orabi, E. Orisakwe, D. Wee, B. Fontaine, R. Gautier, J.-F. Halet, and M. Fornari, M. Fornari, and M. Buongiorno Nardelli, Accurate Prediction of high thermoelectric potential in AMN2 tight-binding Hamiltonian matrices from ab initio callayered nitrides: electronic structure, phonons, and anculations: Minimal basis sets, Phys. Rev. B 93, 035104 harmonic effects, J. Mater. Chem. A 3, 9945–9954 (2016). (2015). [34] L. A. Agapito, M. Fornari, D. Ceresoli, A. Ferretti, S. Curtarolo, and M. Buongiorno Nardelli, Accurate [46] R. L. Henderson, Job scheduling under the Portable Batch System (Springer Berlin Heidelberg, Berlin, HeiTight-Binding Hamiltonians for 2D and Layered Madelberg, 1995), pp. 279–294. terials, Phys. Rev. B 93, 125137 (2016). [35] L. A. Agapito, S. Curtarolo, and M. Buon- [47] G. Farault, R. Gautier, C. F. Baker, A. Bowman, and giorno Nardelli, Reformulation of DFT + U as a PseuD. H. Gregory, Crystal Chemistry and Electronic Strucdohybrid Hubbard Density Functional for Accelerated ture of the Metallic Ternary Nitride, SrTiN2, Chem. Materials Discovery, Phys. Rev. X 5, 011006 (2015). Mater. 15, 3922–3929 (2003).

12

[48] D. H. Gregory, M. G. Barker, P. P. Edwards, M. Slaski, [52] G. A. Slack and R. G. Ross, Thermal conductivity unand D. J. Siddons, Synthesis, Structure, and Magnetic der pressure and through phase transitions in solid alProperties of the New Ternary Nitride BaHfN2 and kali halides. II. Theory, J. Phys. C: Solid State Phys. of the BaHf1−x Zrx N2 Solid Solution, Journal of Solid 18, 3957 (1985). State Chemistry 137, 62–70 (1998). [53] Y. Michihiro, K. Itsuki, S. Endou, K. Nakamura, and T. Ohno, Effects of the multipole polarization on the [49] I. Ohkubo and T. Mori, Two-Dimensional Layered elastic constants and ionic conductivity in cubic strucComplex Nitrides as a New Class of Thermoelectric ture crystals, Solid State Ion. 181, 572–577 (2010). Materials, Chem. Mater. 26, 2532–2536 (2014). [50] D. H. Gregory, M. G. Barker, P. P. Edwards, and D. J. [54] P.-O. L¨owdin, Quantum Theory of Many-Particle Systems. II. Study of the Ordinary Hartree-Fock ApproxiSiddons, Synthesis and Structure of the New Ternary mation, Phys. Rev. 97, 1490–1508 (1955). Nitride SrTiN2, Inorg. Chem. 37, 3775–3778 (1998). [51] A. A. Averkin, Y. A. Logachev, A. V. Petrov, and N. S. Tsypkina, Thermoconductivity of alkali-halide crystals under pressure, Fizika Tverdogo Tela 19, 1692–1701 (1977).

[55] U. Schr¨oder, A new model for lattice dynamics (“breathing shell model”), Solid State Commun. 4, 347– 349 (1966).

13